DSS Phase Transformation Ioaw
Embed Size (px)
Transcript of DSS Phase Transformation Ioaw
FINAL REPORT on
CLEAN CAST STEEL TECHNOLOGY: DETERMINATION OF TRANSFORMATION DIAGRAMS FOR DUPLEX STAINLESS STEEL.
By DR. L.S. CHUMBLEY IOWA STATE UNIVERSITY
THE DEPARTMENT OF ENERGY, And THE STEEL FOUNDERS SOCIETY OF AMERICA
DOE CONTRACT N0. DE-FC36-02ID14229
REPORT NO. 527992-2005 Project Final Report
CLEAN CAST STEEL TECHNOLOGY: DETERMINATION OF TRANSFORMATION DIAGRAMS FOR DUPLEX STAINLESS STEEL. ABSTRACT Duplex stainless steels (DSS) constitute both ferrite and austenite as a matrix. Such a microstructure confers a high corrosion resistance with favorable mechanical properties. However, intermetallic phases such as sigma () and chi () can also form during casting or high-temperature processing and can degrade the properties of the DSS. This research was initiated to develop time-temperature-transformation (TTT) and continuous-cooling- transformation (CCT) diagrams of two types of cast duplex stainless steels, CD3MN (Fe 22Cr-5Ni-Mo-N) and CD3MWCuN (Fe-25Cr-7Ni-Mo-W-Cu-N), in order to understand the time and temperature ranges for intermetallic phase formation. The alloys were heat treated isothermally or under controlled cooling conditions and then characterized using conventional metallographic methods that included tint etching, and also using electron microscopy (SEM, TEM) and wavelength dispersive spectroscopy (WDS). The kinetics of intermetallic-phase ( + ) formation were analyzed using the Johnson-Mehl-Avrami (JMA) equation in the case of isothermal transformations and a modified form of this equation in the case of continuous cooling transformations, The rate of intermetallic-phase formation was found to be much faster in CD3MWCuN than CD3MN due mainly to differences in the major alloying contents such as Cr, Ni and Mo. To examine in more detail the effects of these elements of the phase stabilities, a series of eight steel castings was designed with the Cr, Ni and Mo contents systematically varied with respect to the nominal composition of CD3MN. The effects of varying the contents of alloying additions on the formation of intermetallic phases were also studied computationally using the commercial thermodynamic software package, Thermo-Calc. In general, was stabilized with increasing Cr addition and by increasing Mo addition. However, a delicate balance among Ni and other minor elements such as N and Si also exists. Phase equilibria in DSS can be affected by local composition fluctuations in the cast alloy. This may cause discrepancy between thermodynamic prediction and experimental observation. GENERAL INTRODUCTION Duplex stainless steels (DSS) constitute a set of steels possessing a nearly equal amount of the ferrite (-Fe) and austenite (-Fe) phases as a matrix. Commercial duplex stainless steels originated in 1933 when the J. Holtzer Company, a French firm, mistakenly made an alloy containing 20%Cr-8%Ni-2.5%Mo rather than the target alloy of 1 8%Cr- 9%Ni-2.5%Mo. Upon investigation of the new alloy, which consisted of a high volume fraction of ferrite in an austenite matrix, it was found that it possessed high intergranular corrosion resistance under various environments. Firms in other countries, such as Sweden and the United States, started to research and produce DSS beginning from the 1940s. The austenite+ferrite matrix is attainable by combining various phase stabilizing elements. Cr and Mo are effective ferrite stabilizers, producing a wide ferrite field in phase diagrams. In general, stainless steels having ferrite as the predominant phase have excellent corrosion resistance due to the high solubility of Cr in ferrite. On the other 2
hand, Ni and N, which are effective austenite stabilizers, increase the austenite region in Fe-based systems and are known to improve mechanical properties. Thus, a structure including high Cr, Mo, Ni and N will produce a favorable combination of mechanical properties and high corrosion - resistance. The effect produced by these alloying elements on corrosion resistance is indicated by the pitting resistance equivalent number (PREN) as shown in Eq. 1. The higher the PREN the better the predicted corrosion properties of a DSS. Alloys having a PREN greater than 40 are categorized as superduplex grade DSS (Fig. 1). PREN=%Cr + 3.3 x %Mo + 17 x %N Eq. 1
Fig. 1. Nominal PREN values for different stainless steels.  DSS alloys are widely used for their high corrosion resistance in severe corrosive aqueous environments at service temperatures up to about 800C. Both wrought and cast DSS alloys are available depending on the application. A tremendous amount of literature has been published regarding the phase transformation behavior, alloying element effects, corrosion resistance and mechanical properties of wrought DSS. However, even though cast DSS are used in many applications, they have been the subject of little research. It should be expected that the phase equilibria are different in the cast and wrought alloys due to differences in their nominal compositions. The research undertaken in this study was to develop time-temperaturetransformation (TTT, also known as isothermal transformation or IT) diagrams and continuous-cooling-transformation (CCT) diagrams for two types of cast DSS alloys, designated CD3MN and CD3MWCuN by the Alloy Casting Institute (ACI). Phase 3
transformations in these alloys follow a nucleation and growth mechanism that is diffusion controlled. The transformation kinetics and phase constituents that occur as a result of quenching followed by isothermal holds were examined and directly measured by optical analysis using standard metallographic techniques. The phase transformation kinetics for both isothermal hold and continuous cooled alloys were analyzed from the experimental data using Johnson-Mehl-Avrami (JMA) analysis. The effects of alloying elements on the phase transformations during heat treatment were interpreted with the aid of the commercial thermodynamic package, Thermo-Calc. Thermo-Calc enables one to determine phase equilibria of metallic systems by using the appropriate thermodynamic databases included in the package. LITERATURE REVIEW Iron-Carbon Alloys (Fe-C Metastable System) The iron-carbon alloy system represents the basis of steels. The reasons for the importance of carbon steels are that they are easily and inexpensively produced and possess a favorable mixture of mechanical properties such as strength, toughness, and ductility by means of casting, machining and heat treating. Such a combination of properties and inexpensive price makes carbon steels attractive in industries and markets. However, the crucial disadvantage of plain-carbon steels is their poor corrosion resistance. Corrosion can be slowed by painting, enameling, or by appropriate alloying additions, such as Cr. When added to a level greater than about 10.5 wt%, Cr protects steels from oxidation (rust) by forming a continuous, Cr-rich passive layer on the metal surface. The iron-carbon binary phase diagram is shown in Fig. 2. Pure iron is able to form in three allotropic variants: alpha (), gamma (), and delta (). Alpha and delta iron have
Fig. 2. Fe-C phase Diagram.
a body-centered cubic (BCC) lattice structure. They are conventionally called ferrite or ferrite depending on the mode of formation. The -Fe phase has a face-centered cubic (FCC) lattice structure and is conventionally called austenite. The crystallographic properties of the different allotropic forms of iron are summarized in Table 1. Table 1. Crystallographic properties of pure iron. 
Carbon atoms occupy interstitial sites in the BCC ferrite and FCC austenite unit cells, and carbon solubility is directly related to hardening of steels. The intermetallic compound of Fe is called cementite and exists at 6.67 wt.%C with negligible solubility limits. Cementite has an orthorhombic lattice structure and is brittle and hard. An invariant reaction known as the eutectoid reaction results in the formation of a lamellar +Fe3C structure during cooling. This two-phase mixture is referred to as pearlite. Since the pearlitic structure consists of soft ferrite and hard cementite layers, favorable mechanical properties can be obtained. Effects of Alloying Additions on Iron-Carbon Alloys The addition of alloying elements to the iron-carbon system affects the stability of the phases. Additions such as Cr, Si, Al, and Mo are called ferrite stabilizers since they promote ferrite phase formation over wider composition and temperature ranges than what are found in the Fe-C system. At the same time, the austenite region is contracted, i.e. the loop shrinks. The gamma loop is seen in the Fe-Cr phase diagram in Fig. 3. In contrast, elements such as C, Ni, Mn and N promote austenite formation and are called austenite stabilizers. The effect of Ni on the stability of the iron phases is shown in the Fe-Ni phase diagram in Fig 4. Zener and Andrews  described phase stabilizing effects in terms of thermodynamic variables. The ratio of alloying element concentrations in the -phase (C) to that in the phase (C) follows an Arrhenius-type relationship (Eq. 2).
where is a constant and H is the enthalpy change, which is equal to the heat absorbed per unit of solute dissolving in the -phase minus the heat absorbed per unit of solute dissolving in -phase, i.e., H = H - H. H is positive for ferrite stabilizers since H is greater than H. In this case, a -loop is introduced. For the austenite stabilizers, if H is
Fig. 3. Fe-Cr phase diagram and enlarged view of gamma loop. smaller than H, H becomes negative, and the -region is expanded. Basic phase diagrams in terms of H are illustrated in Figs. 3 and 4. The relative contribution to the phase-forming strength is shown in Fig. 5.
Fig. 4. Fe-Ni phase diagram and enlarged view of expanded gamma regi